|Monthly Tech-Tip |
Notice the water has wicked up to about 1 cm from the rim (the piece sat in water overnight). The glaze fits so there are no cracks for the water to seep through. However, being fired at cone 04, the body is quite porous. The piece has a unglazed base. Notice the water even travelled up the handle. Less exposed bare clay on the base would improve the situation somewhat, however it would be much better to choose a body that vitrifies sufficiently dense so that it does not absorb water (or fire to a higher temperature). There is a not-so-obvious issue here also: Although this piece did not explode in the microwave, it got incredibly hot. Amazingly, through all of this, the glaze has not crazed. It is G3879.
The commercial cone 04 clear brushing glaze on the left works really well on our bodies so I sent it away to be analyzed (about $130). From that information and using my account at insight-live.com I was able to create a recipe, having the same chemistry, employing two Fusion frits (which amazingly supplied all of the fluxing oxides). In this cone 04 melt fluidity comparison they are almost identical (mine, G3879, has a little more surface tension). The Al2O3 and SiO2 levels would make, even a cone 6 glaze, jealous! So it should be very durable. And it has low thermal expansion (no crazing). With the bucket of dipping-slurry I made I can glaze a piece perfectly evenly in seconds rather than the normal 10 minutes of fiddling with a brush and three coats! I have used it on dozens of pieces, it's amazing. One caution: It is possible to duplicate a transparent glaze like this but not a coloured one (a lab could not analyze the complexities of the color, stain colors are about more than chemistry (firing method, particle physics). For colored glaze you have to do trial-and-error testing with stain additions to this base.
The term vitrified refers to the fired state of a piece of porcelain or stoneware. Vitrified ware has been fired high enough to make it very strong, hard and dense.
Clay Body Porosity
In ceramics, porosity is considered an indication of density, and therefore strength and durability. Porosity is measured by the weight increase when boiled in water.
Microwave safety is a concern in the production of function ceramic ware.
G3879 - Cone 04 Transparent Low-Expansion Base Glaze
A super transparent low fire base clear glaze created by reverse engineering a commercial product.